**University of Naples “Federico II” **

**School of Polytechnic and Basic Sciences **

### Department of Structures for Engineering and Architecture

**Ph.D. Programme in Structural, Geotechnical and ** **Seismic Engineering **

**XXIX Cycle **

### MARIA GRAZIA SIMONELLI Ph.D. Thesis

**PLASTIC BUCKLING OF THIN AND ** **MODERATELY THIN PLATES AND ** **SHELLS: CLASSIC PROBLEMS AND **

**NEW PERSPECTIVES**

### TUTOR: PROF. ING. FEDERICO GUARRACINO

**2017 **

*To my family and Eric *

1

**Acknowledgments **

First of all, I would like to express my sincere gratitude to Prof. Federico Guarracino who followed and supported me during the whole Ph.D. programme and offered me the opportunity to work in an outstanding academic department.

His guidance has given me the chance to develop a more rigorous and critic approach to scientific research and has encouraged me to have more self- confidence about my personal.

I am grateful to Prof. Luciano Rosati for his patience and understanding. His suggestions and practical indications have always incited me to expand my knowledge in the broad field of research. A special thank goes also to Prof. Paolo Budetta for supporting me in experimental research and for having shared his knowledge and time with me.

A particular acknowledgment is due to two persons who have appreciated me.

First, I would like to express my gratitude to Aldo Giordano for trusting me since I was a student. He has understood my passion and determination in the field and, despite the lack of time, he has always taught me more than I could dare to ask.

Also, I wish to thank Francesco Marmo for making me believe in the quality of research, giving me the motivation and the confidence to go ahead and sharing with me his knowledge.

I would like to express my sincere and devoted gratitude to Prof. Carlalberto Anselmi for the initial inspiration. He has motivated me with his profound passion for scientific studies, giving me the methodology and the fundamental knowledges which have made possible my achievements.

A warm acknowledgment is due to my Ph.D. colleagues, Stefania Fabozzi, Fabiana De Serio and Antonino Iannuzzo for their example of perseverance. They have shown me in a friendly manner how to face everyday difficulties in academic life. In particular, special thanks go to my roommate Francesca Linda Perelli for the light-hearted atmosphere and for sharing the passion for mathematics and physics.

2

I would like to thank all the students of the courses of “Analisi Limite delle Strutture” and “Scienza delle Costruzioni” taught by Prof. Federico Guarracino for motivating me to face difficulties, for trusting my advice and my knowledge and for having enriched me with their opinions and doubts about structural engineering problems.

I am particularly grateful to my friend Maria Romano for supporting me all the time with her wise suggestions, in many circumstance she has helped me to improve myself and never give up. Special thanks to Le Socie which encouraged me like sisters: their support has been always felt. They continue to inspire me day by day and make me give my best in both professional and personal aspects of my life.

Last but not least, I would like to thank my mother and my father for giving me the most important nurtures: the determination, the spirit of sacrifice and the willpower to go ahead. They have always strongly supported me in any decision. I would also like to thank my brother and Lilla for their patience and loving support and Eric for the love and the understanding: he is the reason why I go successfully ahead in my life and to him I wish to dedicate this important achievement.

Naples, March 2017

*Maria Grazia Simonelli *

3

**Index **

**Acknowledgments ... 1 **

**List of figures ... 5 **

**List of tables ... 9 **

**Introduction ... 11 **

**1. ** **The theory of plasticity ... 17 **

1.1. Flow and deformation theories of plasticity ... 19

1.2. Constitutive laws and analytical relations in the flow theory of plasticity ... 21

1.3. Constitutive laws and analytical relations in the deformation theory of plasticity ... 35

1.4. Other plasticity approaches ... 39

1.5. Experimental stress-strain curves ... 41

1.6. Uniaxial behaviour ... 47

**2. ** **The “plastic buckling paradox” ... 51 **

2.1. The concept of buckling ... 53

2.2. Bifurcation buckling ... 55

2.3. Elastic buckling ... 57

2.4. Plastic buckling ... 60

2.5. The “plastic buckling paradox” ... 65

2.6. Open issues in the investigation of the plastic buckling paradox ... 76

**3. ** **Plastic buckling of a cruciform column ... 79 **

3.1. Historical background ... 81

3.2. Torsional buckling: canonic results ... 84

3.3. A procedure for the evaluation of the critical load according to the flow theory of plasticity ... 88

3.4. Discussion of the results ... 96

4

**4. ** **Plastic buckling of cylindrical shells ... 113 **

4.1. Historical background... 115

4.2. Buckling of cylindrical shells: an overview ... 117

4.3. Estimation of buckling strength in case of non-proportional loading123 4.4. Discussion of the results ... 131

4.5. The role of the mode switching ... 137

**5. ** **Conclusions ... 149 **

**References ... 153 **

References for Section 1. ... 153

References for Section 2. ... 153

References for Section 3. ... 155

References for Section 4. ... 158

**Appendixes ... 163 **

Appendix 1. Plastic work in Prandtl-Reuss material ... 163

Appendix 2. Description of Ramberg-Osgood stress-strain curve ... 166

5

**List of figures **

Figure 1 - Geometric illustration of associated flow rule ... 23

Figure 2 - Flat and corner plasticity (Chen and Han, 1988) ... 25

Figure 3 – Differences in plastic flow between von Mises and Tresca yield surfaces. ... 26

Figure 4 - Hardening and softening in rate-independent plasticity: motion of yield surface in stress space ... 31

Figure 5 – The concept of slip in single crystal (schematic).(Batdorf and Budiansky, 1949) ... 40

Figure 6 – A loading surface with a corner in stress space. ... 40

Figure 7 – Determination of K and n in the Ramberg-Osgood stress-strain curve. (Jones, 2009) ... 43

Figure 8 - Ramberg-Osgood stress-strain curves for various strain hardening values.(Jones, 2009) ... 44

Figure 9 - Overlap of Ramberg-Osgood and Nadai stress-strain curves for an aluminium alloy. ... 46

Figure 10: Tangent, *E , and secant, *_{t}*E , moduli in a simple tension test... 48 ** _{s}*
Figure 11: Unloading in the

*J*2 flow theory of plasticity. ... 49

Figure 12: Bifurcation buckling. ... 53

Figure 13: Nonlinear collapse. ... 54

Figure 14: Stable symmetric buckling and influence of imperfections. ... 56

Figure 15: Instable symmetric buckling and influence of imperfections. ... 56

Figure 16: Asymmetric buckling and influence of imperfections. ... 57

Figure 17: Critical load for a simply supported and uniformly compressed rod. ... 58

Figure 18: Plate subjected to in-plane compressive loading. (Singer, Arbocz and Weller, 1998) ... 59

Figure 19: Plastic buckling of a cylindrical shell subjected to axial compression. ... 61

Figure 20: Euler’s curve of instability. ... 62

Figure 21: Shanley approach to inelastic column buckling. ... 64

6

Figure 22: Onat and Drucker model (1953). a) simplified geometrical model. b)
simplified material model. ... 67
Figure 23: Hutchinson and Budiansky numerical results for critical load as a
function of imperfection amplitude (1976). ... 68
Figure 24: Modes of buckling of Lee’s tests (1962). ... 68
Figure 25: Batterman hinge model for cylindrical shells (1965). ... 69
Figure 26: Numerical and experimental results fo. specimens (Set A). (Giezen,
Babcock and Singer, 1991) ... 72
Figure 27:Theoretical and experimental results for L/D = 1 cylinders. (Blachut,
Galletly and James, 1996) ... 73
Figure 28:Axisymmetric mode of wrinkling observed by Bardi and Kyriakides
(2006). ... 74
Figure 29:Results of axially compressed imperfect cylinders. (Shamass, Alfano
and Guarracino, 2014). ... 75
Figure 30: Torsional buckling of a cruciform column. ... 84
Figure 31: Cross section of a cruciform column. ... 85
Figure 32: Strain increment for a perfect column according to the flow theory of
plasticity. ... 87
Figure 33: Strain increment for an imperfect ( ) vs a perfect ( ) column
according to the flow theory of plasticity. ... 89
Figure 34: Twisted configuration of an imperfect cruciform column. ... 90
Figure 35: Iterative procedure for the evaluation of the critical twisting load of
an imperfect cruciform column according to the deformation theory of plasticity. 94
Figure 36: Iterative procedure for the evaluation of the critical twisting load of
an imperfect cruciform column according to the flow theory of plasticity. ... 95
Figure 37: Plots of the Ramberg-Osgood curves for the considered aluminium
alloys. ... 98
Figure 38: Non-dimensional plots of the Ramberg-Osgood curves for the
considered aluminium alloys. ... 98
Figure 39: FE model of a cruciform column. ... 100
Figure 40: Plots of different shear moduli versus the compressive stress, for
an imperfection amplitude *1/10h*. ... 102

7

Figure 41: Plots of different shear moduli versus the compressive stress, for
an imperfection amplitude *1/10h*. ... 103
Figure 42: Plots of different shear moduli versus the compressive stress, for
an imperfection amplitude *1/10h*. ... 104
Figure 43: Plots of different shear moduli versus the compressive stress, for
an imperfection amplitude *1/100h*. ... 105
Figure 44: Plots of different shear moduli versus the compressive stress, for
an imperfection amplitude *1/100h*. ... 106
Figure 45: Plots of different shear moduli versus the compressive stress, for
an imperfection amplitude *1/100h*. ... 106
Figure 46: Axial load versus torsional rotation in ABAQUS, imperfection
amplitude: *1/10h*. ... 107
Figure 47: Axial load versus torsional rotation in ABAQUS, imperfection
amplitude: *1/10h*. ... 108
Figure 48: Axial load versus torsional rotation in ABAQUS, imperfection
amplitude: *1/10h*. ... 108
Figure 49: Axial load versus torsional rotation in ABAQUS, imperfection
amplitude: *1/100h*. ... 109
Figure 50: Axial load versus torsional rotation in ABAQUS, imperfection
amplitude: *1/100h*. ... 109
Figure 51: Axial load versus torsional rotation in ABAQUS, imperfection
amplitude: *1/100h*. ... 110
Figure 52: Load-deflection curves showing limit and bifurcation points.

(Bushnell, 1984) ... 116 Figure 53: Cylindrical shell displacements and forces. (Yoo and Lee, 2011) . 118 Figure 54: Cylindrical shells under simple loading conditions: a) axial compression; ... 120 Figure 55:Equilibrium paths of axially compressed cylinder. (Yoo and Lee, 2011) ... 121 Figure 56: Buckling of a cylindrical shell subjected to a non-proportional loading. ... 124 Figure 57: Ramberg-Osgood stress-strain curves of the considered aluminium alloys... 127

8

Figure 58: Dimensions and coordinate system of a cylindrical shell. ... 128

Figure 59:Experimental setting by Giezen et al.. (Giezen, Babcock and Singer, 1991) ... 129

Figure 60:FE model of cylindrical shells... 130

Figure 61: Load arc length paths for specimen S1. ... 134

Figure 62: Lateral pressure-arc length paths for specimen S2. ... 135

Figure 63: Lateral pressure-arc length paths for specimen S3. ... 135

Figure 64: Lateral pressure-arc length paths for specimen S4. ... 136

Figure 65: Representation of first two circumferential modes for specimens S1- S3. ... 138

Figure 66: Representation of circumferential modes for specimens S1-S3. ... 139

Figure 67: Representation of circumferential modes for specimen S4. ... 140

Figure 68: Representation of circumferential modes for specimen S2. ... 140

Figure 69: Lateral pressure-arc length paths for specimen S1. ... 142

Figure 70: Lateral pressure-arc length paths for specimen S2. ... 142

Figure 71: Lateral pressure-arc length paths for specimen S3. ... 143

Figure 72: Lateral pressure-arc length paths for specimen S4. ... 143

9

**List of tables **

Table 1 – Difference between flow and deformation theories of plasticity and

the plastic buckling paradox... 66

Table 2 - Ramberg-Osgood parameters for the considered aluminium alloys. .. 97

Table 3 - Characteristics of the analysed specimens. ... 99

Table 4 - Critical stress for a perfect specimen according to Eqs. (72), flow, and (78), deformation theory of plasticity vs ABAQUS elastic results. ... 100

Table 5 - Results obtained from the procedure proposed in this paper for an imperfection equal to 1/10 of the flange thickness, h, versus FE and experimental ones. ... 101

Table 6 - Results obtained from the procedure proposed in this paper for an
imperfection equal to 1/100 of the flange thickness, *1 / 100 h*, versus FE and
experimental ones. ... 105

Table 7 - Percent differences between the analytical solutions for the two
different values of the imperfection amplitude, *1/10h* and *1/100h*. ... 110

Table 8 - Ramberg-Osgood parameters for the considered aluminium alloys. 126 Table 9 - Characteristics of the analysed specimens. ... 127

Table 10 – Applied axial loads, . ... 129

Table 11 – Calculated limit values of the lateral pressure. ... 132

Table 12 – Influence of the initial imperfection shape and amplitude on the buckling loads. ... 133

Table 13 – Calculated limit values of the lateral pressure for low imperfection amplitudes. ... 134

Table 14 – Elastic buckling modes. ... 139

Table 15 – Results of non-linear buckling analysis for specimen S2. ... 141

Table 16 – Results of non-linear buckling analysis for specimen S2. ... 144

Table 17 – Results of non-linear buckling analysis for specimen S3. ... 145

Table 18 – Results of non-linear buckling analysis for specimen S3. ... 146

10

11

**Introduction **

Elastic-plastic instability of structures is a widespread field which involves a broad category of civil and mechanical engineering problems and allows to investigate a rather large variety of structural problems including: the physical and mechanical characterization of materials, the resistance criteria, the modelling of materials respecting to the main theories of plasticity and the phenomena related to material and geometric nonlinearities especially for thin and moderately thin plates and shells.

The concept of buckling involves a sudden lost in strength of a structure due to its lost in shape. In structural engineering, different types of buckling have been shown depending on its appearance in the elastic or plastic range and on the loading path followed. The aim of this work is to investigate the plastic buckling of plates and shells subjected to different loading conditions with respect to the phenomenon of the “plastic buckling paradox”. In particular, by means of a deep numerical investigation on cylindrical shells with different geometrical and material properties, some limitations about the modern numerical nonlinear analyses conducted by the use of the Finite Elements are highlighted and discussed in detail.

In the study of the elastic-plastic response of structures under certain loading conditions, the first issue to deal with is the knowledge of the material behaviour with the definition of appropriate strain-stress relationships. A well-known way to observe a material behaviour is the uniaxial stress test which produces a simple stress-strain curve, in case of compression or tension only. However, in many cases, particular attention must be pay to the material behaviour under multiaxial states of stress for which defining an appropriate constitutive relation is much more complex. Therefore, it becomes necessary to generalize the stress-strain relationships observed from a simple uniaxial test to more general multiaxial stress states. A large amount of stress-strain curves are considered and represented by use of simplified material models, as the Ramberg-Osgood or Nadai ones.

12

At the same time, the study of the main theories of plasticity is conducted. Since the beginning of the twentieth century, there have been many developments in the study of elastic-plastic behaviour of structures. Accordingly, a large improvement has been made in the study of the theory of plasticity, leading to identify different models for engineering materials based on whether path-dependence is accounted for or not. The plasticity models proposed for metals can be divided into two main groups: the deformation (Hencky-Nadai) and the flow (Lévy-Mises) theories of plasticity. In both of these theories the plastic deformation does not allow volume changes because it is ruled by the second invariant of the stress deviator and, in this respect, the flow and the deformation theories are both called

*J*

_{2}theories of plasticity. The flow theory of plasticity assumes that an infinitesimal increment of strain is determined by the current stress and its increment, that is a path-dependent relationship in which the current strain depends not only on the value of the current total stress but also on how the actual stress value has been reached while the deformation theory of plasticity is based on the assumption that, for continued loading, the state of strain is uniquely determined by the state of stress and, therefore, it is essentially a special path-independent nonlinear constitutive law.

Details on the theories of plasticity and on the constitutive relations are described and discussed in Section 1.

Notwithstanding the fact that the deformation theory lacks of physical rigour
with respect to the flow theory of plasticity, in many engineering problems
involving the inelastic buckling of structures, the deformation theory seems to be
more in agreement with the experimental results. This phenomenon is commonly
known as the “plastic buckling paradox” and shows that the *J flow theory of *_{2}
plasticity brings to a significantly overestimation of the critical load while the *J *_{2}
deformation theory of plasticity seems to obtain more accurate results with respect
to the experimental data. This paradox has existed for many years and has involved
a multitude of controversies, many of them are still to be resolved.

In order to deeply examine the roots of the plastic buckling paradox, several plastic buckling problems for plates and shells are investigated. An important observation is made on the nonlinear character of the plastic buckling from both geometrical and material points of view. From the material point of view, the

13

nonlinearity depends on the nonlinearity of the stress-strain relationship of the material while from the geometrical one, it depends on the geometrical configurations of the structural element before and during the loading process, i.e.

on account of some initial imperfections or of second order effects when large deformations appear. Including nonlinearities in the buckling analysis makes the investigation of the equilibrium paths more elaborate. The effects of nonlinearities are decisive in the prediction of the critical load and also in the definition of the post-buckling behaviour. Details on the plastic buckling phenomenon and several examples about the influence of the nonlinearities are illustrated and discussed in Section 2.

Focusing the attention on the fundamentals of the problem, in Section 3 the case of axially compressed cruciform column showing a torsional buckling is thoroughly analysed. As back as 1953, Onat and Drucker found the plastic buckling paradox: the critical compressive stress predicted by the deformation theory was in a better agreement with the experimental results than that predicted by the flow theory. The reasons for this discrepancy were found in the high value of the shear modulus in the flow theory formula. The solution was investigated by conducting an approximate analysis in which small initial imperfections were taken into account. In this manner, assuming that there existed a very small imperfection in the column, the critical load predicted by the flow theory was found to be reduced significantly, getting itself close to that predicted by the deformation theory.

Nevertheless, in other investigations concerning the plastic buckling of the cruciform column it was seen that, depending on the strain hardening of the material, the initial imperfections have to be too much higher and thus no more compatible with those experimentally measured (Gerard and Becker, 1957, Hutchinson and Budiansky,1976). In this respect, in Section 3 a careful analysis is conducted in order to resolve the discrepancies in the flow theory of plasticity due to the shear modulus and also considering the imperfection sensitivity on account of different strain-hardening materials. A new approach for the evaluation of the critical load according to the flow theory of plasticity is presented in detail.

14

In such a manner, a very good agreement between the results from the flow theory of plasticity and other analytical and experimental results can be obtained also for metals with signiﬁcant strain-hardening without the necessity of accounting large initial imperfections.

In the light of the results achieved with the simple case of the cruciform column, the investigation in the plastic buckling is extended in Section 4 to more complex structures such as cylindrical shells of moderate thickness. There are different loading conditions under which the cylindrical shells show the paradox and often it is not possible to obtain reasonable results either by the use of the flow and the deformation theories of plasticity. Indeed, in the case of nonproportional loading, as for instance in the condition of combined axial tension and external pressure investigated by Giezen and Blachut, both the two theories fail to predict the critical load. However, with the contemporary diffusion of powerful computational instruments able to conduct incremental analyses in the plastic range by the use of the Finite Elements, the discrepancy between flow and deformation theories has been reduced and many problems have been resolved. But a doubt still remains: can a modern incremental analysis naturally avoid the plastic buckling paradox? Is that sufficient?

In Section 4, by examining in depth the case of nonproportional loading it is shown that, contrary to what observed in several studies present in literature, is not much the amount of the initial imperfection to govern the problem as its shape.

Indeed, by conducting several numerical analyses, it may be shown that in some cases an opposite phenomenon occurs, i.e. the deformation theory fails in the prediction of the critical load on account of low initial imperfections. This may be thus called the “inverse buckling paradox”, given that it is the deformation theory to overestimate the critical load while the flow theory results more in accordance with the experimental data. Numerical calculations on cylindrical specimens with different geometry and material have been conducted and finally some limitations of the modern numerical non-linear Finite Element analyses have been discussed.

15

The use of the deformation theory of plasticity in the investigation of the inelastic buckling of plates and shells is still recommended for practical applications. In years, many researchers attempted to revise its formulation including unloading (Peek, 2000) or redefining it as a sequence of linear loadings in the case of nonproportional loading (Jahed et al.,1998).

However, the results of the present dissertation highlight a superior reliability of the flow theory of plasticity in the estimation of the critical load with respect to the commonly used deformation theory, contrarily to what is normally agreed in literature. In fact, by conducting a geometrical and material nonlinear finite element analysis, a very good agreement between numerical and experimental results can be found even in presence of the physically more sound flow theory of plasticity, provided that particular attention is pay to constitutive laws and imperfection amplitudes.

**KEYWORDS: • Plasticity • Flow theory • Deformation theory • Stability **

**• Plastic buckling paradox • Plates • Shells • Non-linear FEA **

16

17

**Section 1. **

**1. ** **The theory of plasticity **

18

19

**1.1. ** ** Flow and deformation theories of plasticity **

Since the beginning of the twentieth century, there have been several developments in the study of elastoplastic behaviour of structures and, accordingly, enormous progress has been made in the theories of plasticity leading to identify different models for engineering materials based on whether path-dependence is accounted for or not. The plasticity models that have been proposed for metals in the strain hardening range can be divided into two main groups: the deformation (Hencky) and the flow (Lévy-Mises) theories of plasticity. In both of these theories the plastic deformations do not allow volume changes as plastic yielding is ruled by the second invariant of the deviatoric part of the stress tensor and, in this respect, they are both called

*J*

_{2}

*theories of plasticity.*

Deformation theory was proposed by Hencky in 1924 and subsequently developed around 1945 by the Russian school of Nadai and Ilyushin. This theory of plasticity is essentially based on the assumption of a relationship between stress and strain in global terms, and basically refers to the loading processes that do not involve returns in the elastic path of parts of the structure previously plasticized.

Thus, the elastoplastic problem is treated as a kind of nonlinear elastic problem.

However, while in the loading path a nonlinear elastic relationship has the ease of considering total strains in a one-to-one correspondence with total stresses also during plastic deformation, on the other hand upon unloading the main plastic deformation characteristic of irreversibility is not accounted for and this implies that the application of the deformation theory is very limited. In fact this approach can be applicable only to problems of proportional or simple loading, that is a loading in which the ratios among the stress components remain constant, so that no reversal or cyclic loading are allowed, given that no stress history effects can be accounted for.

Conversely, in the flow or “incremental” theory of plasticity, strain increments are related to stress increments and there are irreversible plastic deformations because of the energy dissipation and, as a consequence, the stress history effects are accounted for. In this manner, at the end of each loading process that leads the material to plasticity, the total strain increment can be decomposed in the sum of two parts, elastic and plastic, so that in the unloading phase the elastic deformation

20

is completely reversible while the plastic one is irreversible and given in value by the difference between the total and the elastic part. The incremental approach has proved to be more effective in describing the non-holonomic nature of the elastic- plastic behaviour of metals, i.e. the final strain is dependent not only on the final value of the load but also on the loading path, and it is extensible to generic loading processes, including reversal or cyclic loading.

In conclusion, while the deformation theory of plasticity is based on the assumption that for continued loading the state of strain is uniquely determined by the state of stress and, therefore, it is essentially a special path-independent non- linear constitutive law, the flow theory of plasticity assumes that an infinitesimal increment of strain is determined by the current stress and its increment, that is a path-dependent relationship in which the current strain depends not only on the value of the current total stress but also on how the actual stress value has been reached.

Finally, it is clear that the incremental theory of plasticity is more in agreement with the experimental behaviour of engineering materials than the deformation theory, and hence more widely applicable. However, that generality and applicability collide with a much higher analytical complexity in calculations.

Notwithstanding the fact that there is a general agreement that the deformation theory of plasticity lacks of physical rigour in comparison to the flow theory, the use of deformation theory is thus practically motivated by the capacity to solve certain problems without the mathematical complications of the flow theory and moreover, in the case of plastic buckling problems of elements under multiaxial stress, the use of deformation theory has been repeatedly reported to predict buckling loads that are in better agreement with the experimental results.

21

**1.2. ** **Constitutive laws and analytical relations in the flow **
**theory of plasticity **

The study of the elastic-plastic response of structures under certain load conditions is a rather complex problem that requires a deep knowledge of the material behaviour under applied loads and, as well, its translation in mathematical terms with an appropriate stress-strain law. A customary way to observe a material behaviour is the uniaxial stress test which leads to a simple stress-strain curve, in case of compression or tension stress state only. However, in order to predict the behaviour of the material under any general combined stress state, it is necessary to understand how to generalize the simple stress-strain relationships observed from an uniaxial test into a more general multiaxial stress states. One-dimensional curves of the constitutive relation that are in accordance with the principal elastic- plastic behaviours highlighted by laboratory experiments show a first elastic linear part and then, above the point of yielding, a nonlinear plastic part. The elastic limit in uniaxial case is well identified by the yielding stress

###

*only, above which the material is considered in plastic range. For a material under all possible combinations of stresses a yield function in terms of stress tensor in the indicial form can be defined as:*

_{y}( * _{ij}*) (

*) 0*

_{ij}*f*

###

*F*

###

*k*(1)

This relationship, in the stress space ( * _{I}*,

*,*

_{II}*), provides the geometrical representation of a yield surface. The term*

_{III}*F*(

###

*) is function of the stresses and*

_{ij}*k*is a parameter which expresses the limit properties of the material in multiaxial states of stress and it may be obtained particularizing the results from the uniaxial case with known experimental results or by more sophisticated triaxial tests. The

( * _{ij}*)

*f*

###

yield function is assumed differentiable so the tangent hyperplane exists at every point belonging to the surface. Considering, in the first instance, an elastic- perfectly plastic material, plastic deformation occurs as soon as the stress vector reaches the yield surface. Continuing the loading above the yielding, for the perfectly plastic equilibrium the increment of stress*d*

###

*has to remain tangent to the yield surface and the plastic flow continues showing a plastic strain increment*

_{ij}22

vector

*d*

_{ij}*normal to the yield surface. In unloading process, the stress state returns inside the yield surface and the irreversible plastic deformation remains constant and all the increments in deformation are purely elastic.*

^{p}During the loading process the condition of plastic flow is:

### (

_{ij}### ) 0

*f*

and *0*

_{ij}*ij*

*df* *f* *d*

(2)

while during the unloading process the condition of elastic return is:

### (

_{ij}### ) 0

*f*

and *0*

_{ij}*ij*

*df* *f* *d*

(3)

At any loading step, in the flow theory an infinitesimal increment of strain is
determined by the current stress and its increment and, recalling that the total strain
increment *d*

###

*satisfies the additive decomposition property, it can be written as the sum of the elastic and plastic strain increments:*

_{ij}*e* *p*

*ij* *ij* *ij*

*d* *d* *d*

(4)
In this manner, the elastic strain increment may be directly derived by differentiating the elastic potential function

### ( )

_{ij}*with respect to stresses*

^{e}###

*, recalling that in the elastic path:*

_{ij}*e*
*e* *ij*
*ij*

*d* *d*

^{ and } ^{ij}_{ij}^{e}

(5)

Similarly, for the plastic strain increment, in 1928 von Mises proposed the
concept of the plastic potential function *g*(

###

*), which frequently assumes the form of*

_{ij}*g* (

_{ij}### ) *J*

_{2}, where

*J is the second invariant of the stress deviator.*

_{2}Therefore the plastic strain increment can be expressed by the equation:

*p*
*ij*

*ij*

*d* *d* *g*

(6)

23

where

*d*

is a positive scalar function which is nonzero only at yielding, that
is when plastic deformation occurs. Eq.(6) defines the plastic flow rule that
postulates an important kinematic assumption for the plastic deformation tensor. It
naturally gives the magnitude of the plastic strain tensor components and implies
that the plastic flow vector *d*

_{ij}*, geometrically represented by a vector with nine components in strain space ( *

^{p}*,*

_{I}*,*

_{II}*) is directed along the normal to the surface of plastic potential*

_{III}*g*(

###

*), when plotted as a free vector in stress space*

_{ij}### (

_{I}### ,

_{II}### ,

_{III}### )

.Another important consequence of this flow law which involves a plastic potential function

*g* (

_{ij}### ) *J*

_{2}dependent only on the stress deviator, is that the volume deformation is purely elastic which is in agreement with experimental evidence. Indeed, it has been generally observed that in metals the largest amount of plastic deformation is due to changes in shape accompanied by very slight, if any, changes in volume. Consequently, the stress deviator does most of the work because of the prevalently distortional nature of plastic deformation. Furthermore, it is worth to underline that plastic deformation is assumed to be rate insensitive.

This assumption implies that all plastic processes are considered to be infinitely slow thus the constitutive equations for plastic deformation may be homogeneous in time and the viscous effects may be neglected.

*Figure 1 - Geometric illustration of associated flow rule *

24

When using the plastic potential theory, the main problem is how to assume the
plastic potential *g*(

###

*), given that the effective form of the function*

_{ij}*g*(

###

*) is undetermined. A simple approach in plasticity theory is to consider that the plastic potential function and the yield function coincide, i.e.*

_{ij}*g*(

###

*)*

_{ij}*f*(

###

*):*

_{ij}*p*
*ij*

*ij*

*d* *d* *f*

(7)

and the direction of the plastic strain increment is thus coincident with the normal to the yield surface at the current stress (see Figure 1), in the coincident stress and strain space

### (

_{I}### ,

_{II}### ,

_{III}### ) ( ,

_{I}

_{II}### ,

_{III}### )

. This simplified equation is called the “associated flow rule” because the plastic flow is no more related to an any unknown potential function but it is associated with a precisely yield criterion function, chosen on the base of the material behaviour. Conversely, if( * _{ij}*) (

*)*

_{ij}*g*

###

*f*

###

the plastic flow follows a “non-associated flow rule”.This simplification is very useful in practical applications since, particularly for materials such as metals, it is possible to choose an adequate yielding surface that agrees with either the constitutive law and the experimental evidence. In this respect, the most widely used criterion for metals is the von Mises yield criterion that has a large applicability not only for its adherence to the real behaviour of the material but also for the regular shape of its surface. Indeed, one has to be very careful in the choice of the surface because in some cases phenomena of corner or flat plasticity may occur (see Figure 2).

25

*Figure 2 - Flat and corner plasticity (Chen and Han, 1988) *

These two phenomena take place on account of the geometry of yielding surface. In fact, on regions of the domain with the same tangent plane the flat plasticity occurs, i.e. the same plastic deformation increment

*d*

_{ij}*corresponds to different stress states while if the surface has some angular points the corner plasticity occurs, i.e. there are different plastic strain increments corresponding to a unique state of stress*

^{p}###

*.*

_{ij}Both flat and corner plasticity phenomena are particularly evident in Tresca
yielding surface, a criterion widely used for metals on account of its more
restrictive nature with respect to von Mises’one, but not as effectively applicable in
plasticity. In fact, considering a plane representation in ( * _{I}*,

*)( *

_{II}*,*

_{I}*) it may be seen that due to the geometry of the Tresca surface on the planes normal to the principal axes *

_{II}*,*

_{I}*and *

_{I}*,*

_{II}*the flat plasticity occurs while at the corners of the domain the corner plasticity occurs. This doed not happen in the case of von Mises surface because of its elliptic shape. In fact, at any point, there is an unique correspondence between the stress state*

_{II}###

*and the plastic strain increment*

_{ij}*d*

_{ij}

^{p}(see Figure 3).

26

*Figure 3 – Differences in plastic flow between von Mises and Tresca yield surfaces. *

Due to the irreversible character of the plastic deformation, the increment of plastic work cannot be recovered. This implies that whenever a change of plastic strain occurs the work of the stresses on the increment of plastic strain must be positive and this condition leads to the convexity of the yield surface and to the normality of the plastic flow:

*p* *p* 0

*ij* *ij* *ij*

*ij*

*dW*

###

*d*

*d*

###

*f*

###

(8)

where the gradient of the yield function _{f}

*ij*

*f* *f*

**n** coincides with the
normal to the yield surface. This convexity of the yield surface implies that the
scalar product of the stress vector and the normal to the yield surface is non-
negative, so that this two vectors must form an angle not larger than

2_{. }

Furthermore, it is opportune to underline that also the undetermined factor

*d*

is related to the magnitude of the increment of plastic work *dW** ^{p}*. The scalar
multiplier

*d*

must always be positive when plastic flow occurs in order to assure
the irreversibility of the plastic deformation and it can be evaluated combining the
stress-strain relation with the consistency condition.
27

In particular, expressing the constitutive relation in terms of stress increments in explicit form:

### (

^{p}### )

*ij* *ijhk* *hk* *hk*

*d* *C* *d* *d*

(9)
and combining it with the consistency condition which maintains the stress
increment vector tangent to the yielding surface, that is the scalar product between
*the stress increment and the gradient of f is zero, it is:*

0

*df * * _{ij}* 0

*ij*

*f* *d*

(10)

where the scalar factor

*d*

can be obtained substituting the stress increment of
the Eq. (9) in Eq. (10):
*ijhk* *hk* *ijhk* 0

*ij* *hk*

*f* *f*

*C* *d* *C* *d*

(11)

and finally:

*ijhk* *hk*

*ij*

*lmno*

*lm* *no*

*f* *C* *d*

*d* *f* *f*

*C*

###

###

###

(12)

where all indices are dummy ones, confirming the scalar character of

*d*

.
Therefore, given the yield function and defined the strain increments, the scalar
multiplier *d*

can be uniquely determined. In this form, the scalar factor *d*

may
be substituted in the Eq.(13) of the constitutive relation:
*ijpq* *rshk*

*pq* *rs*

*ij* *ijhk* *hk*

*lmno*

*lm* *no*

*f* *f*

*C* *C*

*d* *C* *d*

*f* *f*

*C*

###

###

###

(13)

28

and finally the elastic-plastic tensor of tangent moduli for an elastic-perfectly plastic material can be written as:

*ijpq* *rshk*

*pq* *rs*

*EP*

*ijhk* *ijhk*

*lmno*

*lm* *no*

*f* *f*

*C* *C*

*C* *C*

*f* *f*

*C*

###

###

(14)

The generical formulation of the associated flow rule can be hence
particularized considering the simplest form of the von Mises yield criterion. As
previously mentioned, the term *F*(

###

*) in Eq.(1) results dependent on the second invariant of the stress deviator and thus substituting the expression*

_{ij}*F J*(

_{2})

*J*

_{2}in Eq.(1), the plastic potential function becomes:

2

### (

_{ij}### )

2### 0

*f* *J* *k*

(15)
The flow rule in Eq. (7) as well can be written in the simple form:
*p* 2

*ij* *ij*

*ij*

*d* *d* *J* *d s*

(16)

where *s** _{ij}* is the deviatoric stress tensor and

*d*

is the factor of proportionality
with the value:
0
*d*

###

^{}

_{}

^{}0

wherever 0 0

0

*f* *or* *f*

*f*

and 0

0
*df*
*df*

(17)

for an elastic-perfectly plastic material model. The flow rule in Eq. (16) can also be expressed in terms of the components of the strain increments and stresses as:

2 2 2

*p* *p* *p*

*p* *p* *p*

*y* *yz* *xy*

*x* *z* *zx*

*x* *y* *z* *yz* *zx* *xy*

*d* *d* *d*

*d* *d* *d*

*s* *s* *s* *d*

(18)

29

These simplified expressions of the stress-strain relations, Eq.(16) or Eq.(18), are known as the Prandtl-Reuss equations after Prandtl who, in 1924, extended the earlier Levy-von Mises equations and Reuss who, in 1930, extended the Prandtl equations to the three-dimensional case and formulated their general form.

As meaningful consequences, it may be noted that a small increment of plastic strain

*d*

_{ij}*depends only on the current state of the stress deviator*

^{p}*s*

*and not on the total stress increment*

_{ij}*d*

###

*which is required to reach that state and to maintain the plastic flow. Also, the principal axes of stress*

_{ij}###

*(or*

_{ij}*s*

*) and the plastic strain increment are coincident by means of the scalar factor*

_{ij}*d*

. The Prandtl-Reuss
equations confirm that there is no volume change during the plastic flow. In fact,
by Eq. (16) it is easy to note that the plastic volumetric deformation results equal to
zero:
*p* 0

*ii* *ii*

*d*

###

^{}

*d s*

###

^{}(19) Conclusively, it is possible to specify the previously mentioned relation between the undetermined factor

*d*

and the increment of plastic work *dW .*

*Recalling that in incremental theory of plasticity the total strain increment*

^{p}*d*

###

*is the sum of the elastic and plastic strain increments, as seen in Eq.(4), the elastic strain increment can be deduced from Hooke’s law:*

_{ij}*e*

*ij* *ijhk* *hk*

*d* *D d*

(20)
where *D*

*is the tensor of the elastic moduli, or in other terms:*

_{ijhk}2 9

*e* *ij* *kk*

*ij* *ij*

*ds* *d*

*d* *G* *K*

###

###

(21)and the plastic strain increment can be obtained from the previous flow rule.

30

Thus, combining Eq.(21) and (16), the complete stress-strain relation for an elastic-perfectly plastic material can be expressed as:

2 9

*ij* *kk*

*ij* *ij* *ij*

*ds* *d*

*d* *d s*

*G* *K*

###

###

###

(22)in which the unknown term

*d*

is related to the amount of the current
increment in the work of plastic deformation *dW*

*by:*

_{p}2 2

*dW**p*

*d*

###

*k*(23)

which is obtained by simply derivating the rate of plastic work for a Prandtl-
Reuss material (see Appendix 1). By recalling the second invariant of the stress
deviator, *J*_{2} 1 2*s s** _{ij ij}*, and that for a flow rule associated with the von Mises yield
criterion it is also

*J*

_{2}

*k*

^{2}, it is:

### 2

2*p*

*p* *ij* *ij*

*dW* *d* *d k*

(24)
These formulae hold true for an elastic-perfectly plastic material, as said before.
On the other hand, in the case of materials with isotropic hardening, the stress increment allows the yield surface expand homothetically in the stress space for any loading increment. This behaviour of the yield surface in the stress space corresponds to the positive slope of the stress-strain curve in the uniaxial state of stress. Similarly, if the uniaxial stress-strain curve in the plastic range has no slope, the material is elastic-perfectly plastic and the yield surface unchanges during the plastic flow while for an uniaxial stress-strain curve with softening the yield surface above the yielding contracts (see Figure 4).

31

*Figure 4 - Hardening and softening in rate-independent plasticity: motion of yield surface in *
*stress space *

In the light of this similarity between the uniaxial and the multiaxial behaviours, the conditions of hardening in the stress space related to the motion of the yield surface (expanding, constant and contracting) was generalized from the uniaxial stress-strain curves by Drucker in 1950. In particular, he stated that considering a single stress component and the corresponding increment of plastic deformation

*d**p*, the conditions of hardening was:

*p* 0

*d d* for positive hardening with expanding surface

*p* 0

*d d* for perfect plasticity with constant surface

*p* 0

*d d* for softening with contracting surface (25)
For isotropic hardening materials, the yield function depends not only on the
stress tensor * _{ij}* but also on some hardening parameters which constitute internal
variables of the material deduced by experimental evidence.

32

In particular, if the material plasticity is independent on hydrostatic pressure and depends on only one hardening parameter, the yield function may be expressed by:

### (

_{ij}### ) (

_{ij}### ) ( ) 0

*f* *F* *k*

(26)
where is the hardening parameter and ( )*k* is a monotonically increasing
function of . The parameter characterizes the hardening and it depends on the
loading process, in particular on the energy dissipated in the straining process.

Until the first yield surface is attained, the hardening parameter is a constant (as seen in the case of elastic-perfectly plastic material with the Eq.(1)) and successively, once plastic deformation occurs, it increases and makes the yield surface expand to a larger one in case of positive hardening material. If the loading process is first reversed and successively reapplied, plasticity is attained on the expanded surface.

In the case of von Mises yield criterion, the term *F*(

###

*) is a function of the second invariant of the stress deviator,*

_{ij}*F*(

###

*)*

_{ij}*F J*(

_{2})

*J*

_{2}, and the yield function in Eq. (26) results:

2

### (

_{ij}### )

2### ( ) 0

*f* *J* *k*

(27)
where the unknown terms are the hardening parameter and the hardening
function ( )*k* .

In order to obtain the hardening parameter , two types of assumption are generally made: the strain-hardening or the work-hardening. The choice of one of these hypothesis for the determination of the hardening parameter depends on the constitutive relation characterizing the material and on the yield criterion adopted.

The strain-hardening assumption is easier to apply than the work-hardening one and for this reason it is used in most applications. Incidentally, by using the von Mises yield criterion and assuming the constitutive Prandtl-Reuss equations, the strain-hardening and the work-hardening assumptions lead to equivalent results so that the strain-hardening assumption can be chosen to evaluate the hardening

33

parameter . For the strain-hardening assumption, the hardening parameter can be determined as a function of the total equivalent plastic strain. In this manner, it is introduced as:

*p* *p*

*eq* *d* *eq*

###

###

(28) Under this assumption, an important observation is that the measure of the hardening parameter does not depend upon the strain path but only on the initial and final points of the strain flow in the plastic strain space. The increment of the equivalent plastic strain*d*

_{eq}*in Eq. (28) can be described as:*

^{p}2 1 3 2

*p* *p* *p*

*eq* *ij* *ij*

*d*

###

*d*

###

*d*(29)

and likewise the increment of the hardening parameter

*d*

can be obtained by
recalling that the normality condition holds by the Eq. (7), and that the increment
of plastic deformation follows an associated (von Mises) flow rule:
2 6

*p*
*eq*

*ij* *ij*

*f* *f*

*d* *d* *d*

(30)

where the only unknown term is the scalar multiplier

*d*

which can be
calculated in a manner analogous to what has been shown before. Therefore, by
virtue of Eq. (30), since the multiplier *d*

is determined, the increment of the
hardening parameter in the loading path can be obtained.
On the other hand, in the Eq. (27) the unknow function ( )*k* has to be defined
and it is sufficient to make reference to the uniaxial state of stress. For uniaxial
tension only, the hardening function can be obtained from the uniaxial stress-strain
curve in the plastic range and the equation of the yield surface can be simply
expressed as:

( * ^{p}*)

*k* (31)

34

In such a way, the hardening function depends on the plastic strain (*k* * ^{p}*). As
in the determination of the hardening parameter , by replacing the plastic strain

*p* with the equivalent plastic strain

###

_{eq}*and using a von Mises yield surface, the expression for the expanding yield surface due to isotropic strain-hardening is obtained by:*

^{p}2 2

### (

_{eq}

^{p}### )

*J* *k*

(32)
As previously mentioned, also in the case of isotropic hardening the
undetermined factor *d*

can be found by combining the stress-strain relation with
the consistency condition as done for perfect plasticity. In particular, it is:
0

*df * _{ij}_{p}_{eq}* ^{p}* 0

*ij* *eq*

*f* *dk*

*d* *d*

*d*

(33)

And, by substituting the definition in Eq. (29) for the increment of the equivalent plastic strain, it follows that:

2 0

*ij* *p* 6

*ij* *eq* *ij* *ij*

*f* *dk* *f* *f*

*d* *d*

*d*

(34)

Thus, rearranging the terms, the proportionality scalar factor

*d*

can be written
as:
2 6

*ij*
*ij*

*p*

*eq* *ij* *ij*

*f* *d*

*d* *dk* *f* *f*

*d*

###

###

###

(35)

It may be useful to observe that the terms:

ˆ

*ij*

*f*

*ij* *ij*

*f*

*f* *n*
*f* *f* *f*

###

###

(36)

35

correspond to the unit normal to the yield surface. Thus, by substituting this formula into Eq. (35), the scalar function

*d*

simplifies as:
6 ˆ 2

*f* *ij*

*p*
*eq*

*d* *n d*

*dk*
*d*

(37)

In this compact form, the term

*d*

can be replaced in the constitutive relation
which has a similar expression to the one used for the elastic-perfectly plastic
material in Eq.(9). Indeed, the stress-strain relation for isotropic hardening material
can be expressed in the form:
6 ˆ

2

*ij* *ijhk* *ijlm* *f* *nohk* *hk*

*p* *no*
*eq*

*d* *C* *C n C* *f* *d*

*dk*
*d*

###

###

(38)

where the elastic-plastic tensor of tangent moduli for an isotropic hardening material is found as:

6 ˆ

2

*EP*

*ijhk* *ijhk* *ijlm* *f* *nohk*

*no*
*p*

*eq*

*C* *C* *C* *n C* *f*

*dk*
*d*

(39)

**1.3. ** **Constitutive laws and analytical relations in the **
**deformation theory of plasticity **

As said in Section 1.1., the deformation theory of plasticity is essentially a nonlinear stress-strain relationship. Using the additive decomposition property also in this circumstance, the total strain tensor can be expressed by the sum of the elastic and plastic tensors:

*e* *p*

*ij* *ij* *ij*

(40)

36

where the elastic part is governed by Hooke’s law and the plastic part is much simple with respect to its counterpart in the flow theory of plasticity. The Hencky- Nadai deformation theory for initially isotropic materials, in fact, proposes that the total plastic strain is merely proportional to the stress deviator, so that:

*p*

*ij* *s**ij*

(41)

where is a scalar which may be considered a function of the invariant *J . *_{2}
The Hencky-Nadai equation (41) is similar to Prandtl-Reuss equation (16) except
for the use of the total plastic strain _{ij}* ^{p}* instead of the incremental plastic strain

*p*

*d**ij*. The important property of coaxiality between the increment of plastic strain

*p*

*d**ij* and the total deviatoric stress *s** _{ij}* in the incremental theory can be extended to
the deformation theory. Thus, coaxiality between the total plastic strain

_{ij}*and the total deviatoric stress*

^{p}*s*

*and consequently also with total stress tensor*

_{ij}###

*, can be stated. This because the principal axes of the stress deviator tensor*

_{ij}**S**and the total stress tensor

**σ**coincide.

The scalar function (*J*_{2}) is dependent on material properties which can be
determined by experimental uniaxial stress-strain curve and by introducing the
definition of effective stress and effective plastic strain. By multiplying Eq. (41) by
itself, it is:

2

*p* *p*

*ij* *ij* *s s**ij ij*

(42)

and introducing the definition of effective stress and effective plastic strain, respectively, it is:

2

3 3

*ef* *J* 2*s s**ij ij*

and 2

3

*p* *p* *p*

*ef* *ij* *ij*

(43)

In terms of stress, in the uniaxial tension case with

###

*0 and*

_{I}*II* *III* 0

###

###

the effective stress reduces to the stress###

*. In terms of strain, given that the first principal plastic strain is *

_{I}

_{I}*0 while the other two principal*

^{p}